A new ternary derivative of the Laves phases in the Mg-Co-Ga system.
Pavlyuk, Nazar; Dmytriv, Grygoriy; Pavlyuk, Volodymyr; Ciesielski, Wojciech; Rozdzynska-Kielbik, Beata; Indris, Sylvio; Ehrenberg, Helmut; Acta crystallographica Section B, Structural science, crystal engineering and materials 79 (2023) –; doi:10.1107/S2052520623004511

data_2312138
_publ_section_title
;
 A new ternary derivative of the Laves phases in the Mg-Co-Ga system.
;
_journal_issue                   4
_journal_name_full
'Acta crystallographica Section B, Structural science, crystal engineering and materials'
_journal_paper_doi               10.1107/S2052520623004511
_journal_volume                  79
_journal_year                    2023
_chemical_formula_moiety
'0.011(Ga8), 0.012(Ga8), 0.012(Ga8), 0.18(Ga0.20), 0.155(Ga), Co'
_chemical_formula_sum            'Co Ga0.52 Mg0.74'
_chemical_formula_weight         112.70
_space_group_crystal_system      orthorhombic
_space_group_IT_number           63
_space_group_name_Hall           '-C 2c 2'
_space_group_name_H-M_alt        'C m c m'
_audit_creation_method           SHELXL-2014/7
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            32
_cell_length_a                   4.9868(9)
_cell_length_b                   25.959(4)
_cell_length_c                   8.0508(11)
_cell_measurement_reflns_used    640
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      26.370
_cell_measurement_theta_min      2.977
_cell_volume                     1042.2(3)
_computing_cell_refinement       'CrysAlis CCD (Oxford Diffraction, 2008)'
_computing_data_collection       'CrysAlis CCD (Oxford Diffraction, 2008)'
_computing_data_reduction        'CrysAlis RED (Oxford Diffraction, 2008)'
_computing_molecular_graphics    'DIAMOND (Brandenburg, 2006)'
_computing_publication_material  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    'SHELXS-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'Oxford Diffraction Xcalibur3 CCD'
_diffrn_measurement_method       '\w scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0925
_diffrn_reflns_av_unetI/netI     0.0587
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.998
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_h_min       -6
_diffrn_reflns_limit_k_max       32
_diffrn_reflns_limit_k_min       -32
_diffrn_reflns_limit_l_max       10
_diffrn_reflns_limit_l_min       -10
_diffrn_reflns_number            6142
_diffrn_reflns_point_group_measured_fraction_full 0.998
_diffrn_reflns_point_group_measured_fraction_max 0.998
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         26.370
_diffrn_reflns_theta_min         2.977
_diffrn_source                   'fine-focus sealed tube'
_exptl_absorpt_coefficient_mu    23.121
_exptl_absorpt_correction_T_max  0.630
_exptl_absorpt_correction_T_min  0.343
_exptl_absorpt_correction_type   analytical
_exptl_absorpt_process_details   '(CrysAlis RED; Oxford Diffraction, 2008)'
_exptl_crystal_colour            'metallic grey'
_exptl_crystal_density_diffrn    5.746
_exptl_crystal_density_meas      5.73(2)
_exptl_crystal_density_method    volumetric
_exptl_crystal_description       prism
_exptl_crystal_F_000             1657.1
_exptl_crystal_size_max          0.050
_exptl_crystal_size_mid          0.040
_exptl_crystal_size_min          0.020
_refine_diff_density_max         2.357
_refine_diff_density_min         -1.019
_refine_diff_density_rms         0.459
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.903
_refine_ls_matrix_type           full
_refine_ls_number_parameters     56
_refine_ls_number_reflns         640
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.903
_refine_ls_R_factor_all          0.0786
_refine_ls_R_factor_gt           0.0338
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0340P)^2^] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0622
_refine_ls_wR_factor_ref         0.0886
_reflns_Friedel_coverage         0.000
_reflns_number_gt                196
_reflns_number_total             640
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            ra5132sup1.cif
_cod_data_source_block           II-Mg0.74CoGa0.52
_cod_database_code               2312138
_shelx_shelxl_version_number     2014/7
_shelx_res_checksum              30782
_shelx_hkl_checksum              19702
_cod_database_fobs_code 2312138